Open Journal of Civil Engineering, 2012, 2, 22-26 doi:10.4236/ojce.2012.21004 Published Online March 2012 (http://www.SciRP.org/journal/ojce)
Strength of Concrete in Slabs, Investigates along Direction of Concreting
Bohdan Stawiski Institute of Building Engineering, Wroclaw University of Technology Wybrzeze Wyspianskiego, Wroclaw, Poland
Received October 15, 2011; revised November 21, 2011; accepted November 30, 2011
ABSTRACT In theory of concrete it is assumed that concrete composites are isotropic on a macro scale. For example, it is assumed that a floor slabs or a beams strength is identical in all directions and its nonhomogeneity is random. Hence neither calculations of the load-bearing capacity of structural components nor the techniques of investigating concrete in struc-ture in situ take into account to a sufficient degree the fact that the assumption about concrete isotropy is overly opti-mistic. The present research shows that variation in concrete strength along the direction of concreting has not only a qualitative effect (as is commonly believed), but also a significant quantitative effect. This indicates that concrete is a composite which has not been fully understood yet. The paper presents evaluations of ordinary concrete (OC) homogene-ity along component thickness along the direction of concreting. The ultrasonic method and modified exponential heads with a point contact with concrete were used in the investigations [1-3]. Keywords: Concrete; Compressive Strength of Concrete; Non-Destructive
1. Introduction In a building structure there are components which are ex- pected to have special properties but not necessarily in the whole cross section. Components under bending, such as beams and floor slabs are generally compressed in their upper zone and the concretes compressive strength is vital mainly in this zone. The components are usually moulded in the same position in which they later remain in service, i.e. with their upper zone under compression. Concrete in the upper zone is expected to be slightly weaker than in the lower zone, but it is unclear how much weaker [4,5]. Also flooring slabs in production halls are most exposed to abrasion and impact loads in their upper zone which is not their strongest part. It is known from practice that industrial floors belong to the most often damaged build- ing components.
When reinforced concrete beams or floor slabs are to be tested they can be accessed only from their undersides and so only the bottom parts are tested and on this basis conclusions are drawn about the strength of the concrete in the whole cross section, including in the compressed upper zone. Thus a question arises: how large are the er- rors committed in this kind of investigations?
In order to answer the above and other questions, tests of the strength of concrete in various structural compo- nents, especially in horizontally concreted slabs, were car- ried out. The variation of strength along the thickness of the components was analyzed.
2. Research Significance The research results presented in the paper show that the compressive strength of concrete in horizontally formed structural elements varies along their thickness. In the top zone the strength is by 25% - 30% lower than the strength in the middle zone, and it can be by as much as 100% lower than the strength in the bottom zone. The observa- tions are based on the results of nondestructive tests car- ried out on drill cores taken from the structure, and veri- fied by a destructive method. It is interesting to note that despite the great advances in concrete technology, the variation in compressive strength along the thickness of structural elements is characteristic of both old (over 60 years old) concretes and contemporary ordinary concretes.
3. Test Methodology Before Concrete strength was tested by the ultrasonic method using exponential heads with a point contact with concrete. The detailed specifications of the heads can be found in [2,3]. The heads frequency was 40 and 100 kHz and the diameter of their concentrators amounted to 1 mm2). The heads cross section is shown in Figure 1.
In order to determine the real strength distributions in the existing structures, cylindrical cores 80 mm or 114 mm diameter (Figure 2) were drilled from them in the direction of concreting. Then specimens with their height equal to their diameter were cut out of the cores.
Copyright 2012 SciRes. OJCE
B. STAWISKI 23
Figure 1. Ultrasonic probe equipped with exponential concentrator.
Figure 2. Exemplary cores drilled from slabs.
Ultrasonic measurements were performed on the cores
according to the scheme shown in Figure 3. Ultrasonic pulses (pings) were passed through in two perpendicular directions I and II in planes spaced every 10 mm. In this way one could determine how ping velocity varied along the cores height, i.e. along the thickness of the tested component.
In both test directions ping pass times were determined and velocities CL were calculated. The velocities from the two directions in a tested measurement plane were averaged.
Subsequently, specimens with their height equal to their diameter of 80 mm were cut out of the cores. Aver- age ultrasonic pulse velocity CL for the specimens cen- tral zone was correlated with fatigue strength fc deter- mined by destructive tests carried out in a strength tester. For the different concretes different correlation curves with a linear, exponential or power equation were ob- tained. Exemplary correlation curve equations are given below:
232.705 56.03c Lf C (1) 4.6210.1cf L
c Lf C (3)
where: fcthe compressive strength of concrete MPa, CLping velocity km/s. The determined correlation curve was used to calculate
the strength of concrete in each tested core cross section and the results are presented in the form of graphs illus-
Figure 3. Scheme showing how concrete cores drilled from tested structures were tested. trating concrete strength distribution along the thickness of the tested component.
4. Investigation of Concrete Strength Distribution along Direction of Concreting for Different Structural Components
4.1. Investigation of Concrete in Industrial Floors
After Floor in sugar factorys raw materials storage hall Concrete in an industrial floor must have particularly
good characteristics in the top layer. Since it was to be loaded with warehouse trucks and stored sugar beets and frequently washed the investigated concrete floor (built in 1944) was designed as consisting of a 150 mm thick underlay and a 50 mm thick surface layer and made of concrete with a strength of 20 MPa (concrete A).
As part of the investigations eight cores, each 80 mm in diameter, were drilled from the floor. The investigations showed significant departures from the design. The con- crete subfloors thickness varied from 40 to 150 mm. The surface layer was not made of concrete, but of cement mortar with sand used as the aggregate. Also the thick- ness of this layer was uneven, varying from 40 to 122 mm. After the ultrasonic tests specimens with their height equal to their diameter of 80 mm were cut out of the cores. Two scaling curves: one for the surface layer and the other for the bottom concrete layer were determined. A characteristic concrete compressive strength distribu- tion along the floors thickness is shown in Figure 4.
Strength in the upper zone is much lower than in the lower zone: ranging from 4.7 to 9.8 MPa for the mortar and from 13.9 to 29.0 MPa for the concrete layer. The very low strength of the upper layer of mortar is the re- sult of strong porosity caused by air bubbles escaping upwards during the vibration of concrete. Figure 5 shows the specimens porous top surface.
Floor in warehouse hall with forklift truck transport The floor was built in 1998. Cellular concrete was used
as for the underlay and the 150 mm thick surface layer was made of ordinary concrete with fibre (steel wires) rein- forcement (concrete B). Cores 80 mm high and 80 mm in
Copyright 2012 SciRes. OJCE
B. STAWISKI 24
0 10 20 30
Concrete compression strength f c [MPa]
Figure 4. Concrete strength distribution in concrete underlay and in cement mortar floor.
Figure 5. Top layer of floor is most porous and weakest.
diameter were drilled from the surface layer. Ultrasonic measurements and destructive tests were performed as described above. Also the test results were handled in a similar way. An exemplary strength distribution along the floors thickness is shown in Figure 6.
The upper zone strength is by 40% - 60% lower than the lower zone strength. The design grade of concrete was B25. But the concrete reaches this strength as much down as 90 mm from the top surface.
16 21 26 31
Concrete compression strength f c [MPa]
Figure 6. Exemplary concrete compressive strength distri- bution in warehouse hall floor.
4.2. Investigation of Concrete in Old and New Floor Slabs
Building erected in 1942 Concrete (C) in the floor slab of an industrial building
was investigated. Nine cores 80 mm in diameter were drilled from the whole thickness of the floor whose load- bearing layer was 115 mm